Brazilian Dental Journal (2013) 24(4): 326-329 http://dx.doi.org/10.1590/0103-6440201302113
Influence of Volume and Activation Mode on Polymerization Shrinkage Forces of Resin Cements Sergio Kiyoshi Ishikiriama, Rafael Massunari Maenosono, Denise Ferracioli Oda, Juan Fernando Ordóñez-Aguilera, Linda Wang, Rafael Francisco Lia Mondelli
The concern with the polymerization shrinkage of restorative resin composites also applies to resin cements. The aim of this study was to evaluate the influence of volume and polymerization mode on forces generated during polymerization shrinkage (FGPS) of resin cements. Two light-cured resin cements - Variolink II (VL; Ivoclar Vivadent) and Nexus 3 (NX; Kerr) - and two self-cured resin cements - Multilink (ML; Ivoclar Vivadent) and Cement Post (CP; Angelus) - were inserted between two rectangular steel bases (6x2 mm) with distance set at 0.1, 0.3 and 0.5 mm, establishing a variation of volume. These steel bases were attached to a universal test machine with 50 kg load cell and forces (N) were registered for 10 min. Values of maximum forces generated by each material were subjected to two-way ANOVA and Tukey’s test for individual comparisons (a=0.05). VL, NX and CP developed increasing FGPS as the volume of material increased, while ML presented the opposite behavior. It may be concluded that higher volume increases FGPS even with a concomitant decrease of C-factor, unless the resin cements present lower force generation rates as a function of time in combination with a low C-factor, resulting in stress relief and consequently lower values of FGPS.
The evolution of indirect restorative systems has widened their indications (1), increasing the importance of luting procedures that promote adhesion, durability and aesthetics. For this reason, resin cements became even more relevant, since this group of materials provides improved physical properties and aesthetics (2,3). Despite these advantages, the use of resin materials requires some care, especially as regards polymerization shrinkage. Studies with restorative resin composites found that forces generated during polymerization shrinkage (FGPS) can affect the bond strength between tooth and restoration (4) causing cracks, plaque accumulation and even loss of restoration. Some factors can modify or influence the development of FGPS, among which the cavity configuration factor (C-factor), volume of material and polymerization mode have been intensively studied (5-10). Higher C-factor may increase the intensity of FGPS due to the smaller amount of free surface available for stress relief during the polymerization process (6), while higher volume of material may also increase FGPS due to the greater amount of monomers forming polymeric chains (8). Volume is considered especially important for light-cured restorative resin composite, in which the pre-gel phase is shorter and may not allow stress relief even with a lower C-factor. Stress relief is time-dependent, and the shorter time for
Department of Operative Dentistry, Endodontics and Dental Materials, Bauru School of Dentistry, USP - University of São Paulo, Bauru, SP, Brazil
Correspondence: Prof. Dr. Sergio Kiyoshi Ishikiriama, Alameda Octávio Pinheiro Brisolla, 9-75, Vila Universitária, 17012-901 Bauru, SP, Brasil. Tel: +55-14-32358365. e-mail: [email protected]
Key Words: resin cement, dental stress analysis, polymerization.
polymerization process is responsible for generation of higher forces of light-cured resin composites when compared with the self-cured resin composites (11). In this context, the role of volume and polymerization mode on a luting procedure (high C-factor) with resin cement are still not well established, and a better understanding of the effect of these factors on the generation of FGPS is essential to avoid failures caused by disruption of adhesive bonding. The objective of this study was to evaluate the influence of the volume and activation mode on FGPS of resin cements. The tested null hypothesis was that neither the volume nor the activation system of polymerization reaction may influence the FGPS of resin cements.
Material and Methods
This in vitro study involved the analysis of two factors: volume (three levels) and material (four levels). The response variable was determination of the force. Resin cements used in this experiment, their composition and activation modes are listed in Table 1. In order to capture the FGPS of resin cements, two rectangular steel bases (6x2 mm) previously blasted with aluminum oxide were connected to the universal testing machine (Emic DL 500; Emic Equipamentos e sistemas de Ensaios. Ltda, São José dos Pinhais, PR, Brazil) (12). Only Multilink (ML), a ceramic primer without excesses,
Braz Dent J 24(4) 2013
the beginning of force registration was immediately after their insertion between steel bases. During polymerization of resin cements, forces generated between the steel bases were recorded continuously for 10 min, resulting in a chart of force (N) x time (s) (Fig. 2). Values of maximum force generated by each material have been subjected to two criteria analysis of variance with any individual differences pointed by Tukey‘s test (p